Structural, Spectroscopic and Electrochemical Characterisation of Semi-conducting,
Solvated [Pt(NH3)4](TCNQ)2·(DMF)2 and Non-solvated [Pt(NH3)4](TCNQ)2
Jinzhen Lu,A,G Ayman Nafady,A,B,G Brendan F. Abrahams,C Muhammad Abdulhamid,A,D
Bjorn Winther-Jensen,E,F Alan M Bond,A,H and Lisandra L MartinA,H
A School of Chemistry, Monash University, Clayton, Victoria, 3800, Australia
B Current address: Chemistry Department, College of Science, King Saud University, Riyadh,
C School of Chemistry, University of Melbourne, Victoria, 3010, Australia
D Current address: Department of Applied Physics, Chalmers University of Technology,
E Materials Engineering, Monash University, Clayton, Victoria, 3800, Australia
F Current address: Department of Advanced Science and Engineering, Waseda University,
Tokyo 169-8555, Japan
G Joint first authors with an equal contribution.
H Corresponding authors: Email: [email protected] and [email protected]
Australian Journal of Chemistry 2017, 70(9), 997-1005
Table of contents
Figure S1: Experimental and calculated powder XRD diffraction pattern of
[(NH3)4Pt](TCNQ)2 (2) S3
Figure S2. FTIR spectra of [Pt(NH3)4](TCNQ)2·(DMF)2 (1) and [Pt(NH3)4](TCNQ)2 (2) S4
Figure S3. UV-vis spectra of dissolved 1, 2, LiTCNQ and neutral TCNQ in CH3CN S5
Figure S4. Solution phase electrochemistry of 2 S6
Figure S5. Raman spectra of TCNQ and 2 obtained electrochemically S7
Figure S6. Voltammetric evidence for nucleation/growth mechanism S8
Figure S7. Chromoamperometic evidence for nucleation/growth mechanism S9
Figure S8. 1H NMR spectrum of a supernatant solution after 1 is soaked in D2O S10
Figure S9. FTIR spectrum of 1 after being soaked in D2O S11
Table S1. Catalytic properties for several TCNQ(F4)0/1-/2- derived materials S12
Supplementary References S13
Figure S1: Comparison of X-ray powder diffraction pattern of [Pt(NH3)4](TCNQ)2 (2) (blue)
and that calculated from the structure of [Pt(NH3)4](TCNQ)2 (red). S1
Figure S2: FTIR spectrum of solid (a) [Pt(NH3)4](TCNQ)2·(DMF)2 (1) and solid (b)
Figure S3: UV-vis spectra of dissolved [Pt(NH3)4](TCNQ)2·(DMF)2 (1), [Pt(NH3)4](TCNQ)2
(2), compared with dissolved TCNQ1- (from LiTCNQ) and neutral TCNQ in CH3CN
Figure S4: (a) Transient cyclic voltammograms obtained when chemically synthesized
[Pt(NH3)4](TCNQ)2 (2) (from water) is dissolved in acetonitrile (0.1 M Bu4NPF6) using a GC
(1.5 mm) electrode at designated scan rates. (b) Steady-state voltammogram of the same
solution obtained with a 10 µm Pt micro-disk electrode at scan rate of 20 mV s-1.
Figure S5: Raman spectra of solid TCNQ and solid [Pt(NH3)4][TCNQ]2 (2) collected after
reductive electrolysis (15 min) at Eapp = - 0.15 V when a TCNQ-modified ITO electrode
(mechanical attachment method) is in contact with aqueous 0.10 M [Pt(NH3)4](NO3)2
500 1000 1500 2000
Voltammetric Evidence of a Nucleation/Growth Mechanism for the
TCNQ|[Pt(NH3)4](TCNQ)2 solid-solid state interconversion
Cyclic voltammetry provides support for the presence of rate-determining nucleation-growth
kineticsS2-12 in the electrochemically induced TCNQ|[Pt(NH3)4](TCNQ)2 solid-solid state
interconversion processes. This is provided by the detection of current loops (Figure S9) in
the cyclic voltammograms as can be detected upon reversing the direction of the scan at foot
of reduction process when a TCNQ modified electrode is in contact with 0.1 M [Pt(NH3)4]2+
Figure S6: Cyclic Voltammograms obtained under same conditions as in (a) but at a scan rate
of 20 mV s-1, and for the fourth and fifth cycles with the potential switched at the foot of the
reduction wave, which induces a hysteresis loop (as indicated by an arrow).
Chronoamperometric Evidence of a Nucleation/Growth Mechanism
Additional evidence for nucleation/growth kinetics can be obtained from analysis of current-
time (i-t) data obtained from double potential step chronoamperometric experiments. Figure
S7 shows a chronoamperogram obtained by stepping the potential from an initial value (Ei =
350 mV), where no faradaic current is present, to a more negative value (Ered = -50 mV) that
allows reduction of TCNQ into TCNQ1- along with concomitant interaction with
[Pt(NH3)4]2+(aq) to form [Pt(NH3)4](TCNQ)2. After 20 seconds, the potential is stepped back to
Eox = 250 mV to induce oxidation of TCNQ1- back to its neutral form, TCNQ. Current maxima
characteristic for the presence of a rate-determining nucleation-growth process are clearly
observed for both the reduction and oxidation components.
Figure S7: I-t chronoamperometric transient obtained when a GC electrode modified with
TCNQ (mechanical attachment method) is placed in contact with aqueous 0.1 M
[Pt(NH3)4](NO3)2(aq) electrolyte and the potential is stepped from Ei = 350 to Ered = -50 mV for
20 s to induce reduction and then back to Eox = 250 mV to induce oxidation.
Figure S8: The 1H NMR spectrum of the supernatant following soaking a crystal of
[Pt(NH3)4](TCNQ)2·(DMF)2 (1) in D2O after for ~ 30 mins.
Figure S9: (a) FTIR of a crystal of [Pt(NH3)4](TCNQ)2·(DMF)2 (1) after soaking for ~ 30
mins in D2O, (b) Comparison of the FTIR of 2 (red) and 1 after soaking for ~ 30 mins in D2O
Table S1. Assessment of several TCNQ/TCNQF4-derived compounds, in various redox
level, to act as a catalyst for the redox reaction between thiosulfate anions and ferricyanide
ions in aqueous solution. Reaction conditions are described in the main text and .
Cation Soluble in
TCNQ 0 û û This work
'' 1- Li+ ü û 
'' 1- Bu4N+ û û 
'' 1- [Pt(NH3)4]2+ û û This work
TCNQF4 0 û û This work
'' 1- Li+ ü ü 
'' 1- [Pt(NH3)4]2+ û ü 
'' 2- Li+ ü ü This work
'' 2- Pr4N+ û ü This work
S1. H. Endres, H. J. Keller, W. Moroni, D. Nothe and V. Dong, Acta Crys. B, 1978, 34,
S2. S.-I. Terashita, K. Nazumi, Y. Ozaki and S. Takagi, J. Phys. Chem., 1995, 99, 3618-
S3. F. H. Herbstein and M. Kapon, Crystallogr. Rev., 2008, 14, 3-74.
S4. P. G. Gucciardi, S. Trusso, C. Vasi, S. Patane and M. Allegrini, Phys. Chem. Chem.
Phys., 2002, 4, 2747-2753.
S5. A. Nafady, A. P. O'Mullane, A. M. Bond and A. K. Neufeld, Chem. Mater., 2006,
S6. A. Nafady and A. M. Bond, Inorg. Chem., 2007, 46, 4128-4137.
S7. A. M. Bond, S. Fletcher, F. Marken, S. J. Shaw and P. G. Symons, J. Chem. Soc.,
Faraday Trans., 1996, 92, 3925-3933.
S8. A. M. Bond, S. Fletcher and P. G. Symons, Analyst, 1998, 123, 1891-1904.
S9. M. Oyama, R. D. Webster, M. Suarez, F. Marken, R. G. Compton and S. Okazaki, J.
Phys. Chem. B, 1998, 102, 6588-6595.
S10. A. Nafady, A. M. Bond and A. Bilyk, J. Phys. Chem. C, 2008, 112, 6700-6709.
S11. A. Nafady, A. M. Bond, V. Qu and L. L. Martin, J. Solid State Electrochem., 2013,
S12. A. Nafady, A. M. Bond and A. P. O’Mullane, Inorg. Chem., 2009, 48, 9258-9270.
S13. J. Lu, B. F. Abrahams, B. Winther-Jensen, L. L. Martin and A. M. Bond,
ChemCatChem, 2014, 6, 2345-2353.